# Crystal plasticity finite element simulation of crack ... A new method for 3D simulation of crack...

date post

18-May-2020Category

## Documents

view

4download

0

Embed Size (px)

### Transcript of Crystal plasticity finite element simulation of crack ... A new method for 3D simulation of crack...

Computational Materials Science xxx (2014) xxx–xxx

Contents lists available at ScienceDirect

Computational Materials Science

journal homepage: www.elsevier .com/locate /commatsci

Crystal plasticity finite element simulation of crack growth in single crystals

http://dx.doi.org/10.1016/j.commatsci.2014.03.061 0927-0256/� 2014 Elsevier B.V. All rights reserved.

⇑ Corresponding author. Tel.: +33 1 60 76 30 67; fax: +33 1 60 76 31 50. E-mail address: jia.li@mines-paristech.fr (J. Li).

Please cite this article in press as: J. Li et al., Comput. Mater. Sci. (2014), http://dx.doi.org/10.1016/j.commatsci.2014.03.061

J. Li a,⇑, H. Proudhon a, A. Roos b, V. Chiaruttini b, S. Forest a a MINES ParisTech, Centre des matériaux, CNRS UMR 7633, Evry, France b ONERA, The French Aerospace Lab, Châtillon, France

a r t i c l e i n f o a b s t r a c t

Article history: Received 15 December 2013 Received in revised form 24 March 2014 Accepted 27 March 2014 Available online xxxx

Keywords: Crystal plasticity Finite element Crack propagation Adaptive remeshing Single crystals

A new method for 3D simulation of crack growth in single crystals is proposed. From Crystal Plasticity Finite Element (CPFE) computations of a pre-cracked single crystal, a damage indicator based on the accumulated slip, the resolved shear stress and the normal stress on each slip system is calculated at each integration point and for every time increment. The crack growth direction is then determined in 3D by analysing the damage indicator in the region around the crack front. The crack is extended via remeshing at each propagation event. At this point the CPFE computation is restarted, using the new crack configuration. Two examples in BCC single crystals featuring different crystal orientations and slip systems show the crack propagation simulations under monotonic loading over distances comparable to the crystal size and with non-regular crack shape and path.

� 2014 Elsevier B.V. All rights reserved.

1. Introduction

In many industrial cases, the major part of the total fatigue-life of structural components is spent in the regime of initiation and micro-propagation of small cracks. During small fatigue crack growth, the shape and growth rate directly depend on microstruc- tural features. Microstructure-based models of fatigue-life predic- tion were proposed by [1–4], where accumulated plastic slip, resolved shear stress or normal stress to slip planes were supposed to cause crack initiation. The damage variables based on these models were simulated and compared in [5]. However, to date, reliable prediction of 3D small fatigue crack growth paths in metallic polycrystalline materials remains a challenge.

Different numerical methodologies currently exist to simulate fatigue crack propagation in 3D. The X-FEM approach is one of the most popular methods in Linear Elastic Fracture Mechanics (LEFM) without remeshing [6]. Although it was extended to elasto-plastic fracture mechanics, there are still many technical issues to be resolved. An alternative methodology is the Cohesive Zone approach [7]. However, the crack path must usually be known in advance which limits greatly the prediction of complex paths. Continuum damage mechanics can also be used, but it remains computationally expensive [8,9].

The objective of this paper is to introduce a new methodology to simulate efficiently crack propagation in 3D single crystals. CPFE

computations coupled with a post-processing procedure are used to determine the direction of crack growth and to remesh the crack surface adaptatively at each crack propagation event [10]. The damage indicator, which is based on a combination of resolved shear stress and normal stress with respect to the slip plane, and accumulated plastic slip, is computed and evaluated at the crack front for each load increment.

In Section 3, the methodology is presented and showcased on a single crystal with only one slip system loaded in tension. An example of a single crystal with 12 slip systems is presented in Section 4, under tensile loading. The final section presents a discussion and conclusions.

2. Experimental studies

The material of interest is a near beta titanium alloy VST55531 with a B.C.C. crystal structure. The average grain size is 65 lm. The in situ fatigue experiments were carried out at the ESRF (France) using a triangular prismatic pre-cracked sample under load control (not presented here). The maximum loading amplitude corre- sponds to a tensile stress of 500 MPa. The stress ratio rmax=rmin is 0.1. The growth of fatigue crack surfaces in the polycrystalline sample was characterised by X-ray tomography every 2000 cycles [11]. It was observed that cracks initiated from the notch after 28,000 cycles. The average crack growth rate for the first grains crossed by the crack was about 1 nm per cycle. Thus, at each stage of observation, cracks typically propagated over 2 lm and mainly intragranularly along {112} and {110} crystallographic planes of

http://dx.doi.org/10.1016/j.commatsci.2014.03.061 mailto:jia.li@mines-paristech.fr http://dx.doi.org/10.1016/j.commatsci.2014.03.061 http://www.sciencedirect.com/science/journal/09270256 http://www.elsevier.com/locate/commatsci http://dx.doi.org/10.1016/j.commatsci.2014.03.061

2 J. Li et al. / Computational Materials Science xxx (2014) xxx–xxx

the BCC structure. After 46,000 cycles, cracks propagated into the neighbouring grains.

3. Constitutive model and crack growth methodology

3.1. Proposed methodology for crack propagation

In this section, the crack growth methodology is presented on a simplified test case, as shown in Fig. 1. It consists of ½111�ð112Þ single slip crystal, in which the initial crack plane is perpendicular to the loading direction and the slip plane is oriented at an angle of 54.7� with respect to the crack plane, see Fig. 2(b). In Section 4, the method is applied to a single crystal with a crystal orientation measured by X-ray diffraction during the in situ tomographic experiment, in which all the 12 h111if110g slip systems can be activated. The maximum loading applied in the simulations is the same as in the experiments. However, in these simple exam- ples, the CPFE computations are performed under monotonic load- ing instead of fatigue loading because the methodology remains to be applied to complex loading.

Fig. 1 shows the main steps of the crack growth simulation methodology. For each CPFE computation, the damage indicator is computed at all integration points. Then, a post-processing pro- cedure is carried out at the preset increment to evaluate the dam- age indicator around the crack front, on a set of planes orthogonal to the crack front. For each such plane, the origin is defined at its intersection with the crack front. Then, the crack growth direction is selected as pointing from the origin to the location where the damage indicator is the maximum, at a preset distance R0 from the origin. The crack growth distance R0 is fixed as 2 lm in both examples, which corresponds to the average experimentally measured crack growth distance. The parameter R0 is related to material properties, loading amplitude and other experimental conditions. The set of propagation directions along the front is used to create the geometry of the crack propagation area, which is then

Fig. 1. Crack propagation si

Fig. 2. (a) FE mesh of the pre-cracked single crystal and the applied boundary conditions orientation and the single slip system ½111�ð1 12Þ of the example in Section 3.

Please cite this article in press as: J. Li et al., Comput. Mater. Sci. (2014), http:

inserted into the FE mesh of the single crystal, as will be explained in detail in Section 3.4. Then, a new CPFE computation is carried out with the same loading conditions as before. In this paper, to illustrate the methodology, the procedure is repeated until the whole single crystal is broken.

The initial Finite Element (FE) mesh is a pre-cracked single crys- tal with a rectangular crack, as shown in Fig. 2(a). The FE mesh is generated by inserting a crack surface mesh into a single crystal mesh using Z-cracks [15], which is a module of the Z-set FE soft- ware [13]. The insertion procedure is performed by creating the intersection points and edges of the two meshes and then reme- shing the whole mesh. The size of the single crystalline cube is 100 � 100 � 100 lm3, which approximately corresponds to the size of the grain in which the pre-crack is presented in the exper- imental polycrystalline sample.

Regarding the boundary conditions, according to the loading applied in the in situ experiments, a displacement of 0.5 lm is applied monotonically in a time interval of 1 s at the top surface in the vertical tensile direction z, and vertical displacement is blocked at the bottom surface, so that the loading rate _ezz ¼ 5� 10�3 s�1. Detailed boundary conditions are shown in Fig. 2(a). For the single slip crystal, symmetry conditions in the y direction are applied at the back and the front surface to minimise the free surface effect. In the case of 12 slip systems crystal in Sec- tion 4, these surfaces are free of forces since the prediction of free surface effects on cracking and simulation of curved cracks also belong to the objective of this work.

3.2. Crystal plasticity model

In order to analyse the slip system activity and to determine the driving force for short crack propagation, an elasto–visco-plastic crystal plasticity model was selected [12]. The CPFE computations were carried out in the framework of infinitesimal strains using the

mulation methodology.

. The dimension of the mes

*View more*